Journal of Hazardous Materials 168 (2009) 888–894
Contents lists available at ScienceDirect
Journal of Hazardous Materials journal homepage: www.elsevier.com/locate/jhazmat
Removal of ﬂuoride ions from aqueous solution by waste mud Baris Kemer a , Duygu Ozdes a , Ali Gundogdu a , Volkan N. Bulut a , Celal Duran a , Mustafa Soylak b,∗ a b
Karadeniz Technical University, Faculty of Arts & Sciences, Department of Chemistry, 61080 Trabzon, Turkiye Erciyes University, Faculty of Arts & Sciences, Department of Chemistry, 38039 Kayseri, Turkiye
a r t i c l e
i n f o
Article history: Received 16 January 2009 Received in revised form 19 February 2009 Accepted 19 February 2009 Available online 3 March 2009 Keywords: Fluoride Removal Adsorption Waste mud
a b s t r a c t The present study was carried out to assess the ability of original waste mud (o-WM) and different types of activated waste mud which are acid-activated (a-WM) and precipitated waste mud (p-WM), in order to remove excess of ﬂuoride from aqueous solution by using batch technique. The p-WM exhibited greater performance than the others. Adsorption studies were conducted as a function of pH, contact time, initial ﬂuoride concentration, adsorbent concentration, temperature, etc. Studies were also performed to understand the effect of some co-existing ions present in aqueous solutions. Adsorption process was found to be almost independent of pH for all types of waste mud. Among the kinetic models tested for p-WM, pseudo-second-order model ﬁtted the kinetic data well with a perfect correlation coefﬁcient value of 1.00. It was found that the adequate time for the adsorption equilibrium of ﬂuoride was only 1 h. Thermodynamic parameters including the Gibbs free energy (G◦ ), enthalpy (H◦ ), and entropy (S◦ ) revealed that adsorption of ﬂuoride ions on the p-WM was feasible, spontaneous and endothermic in the temperature range of 0–40 ◦ C. Experimental data showed a good ﬁt with the Langmuir and Freundlich adsorption isotherm models. Results of this study demonstrated the effectiveness and feasibility of WM for removal of ﬂuoride ions from aqueous solution. © 2009 Elsevier B.V. All rights reserved.
1. Introduction Fluoride is a natural mineral that is found in many foods and in all waters and wastewaters. Low concentration of ﬂuoride in drinking water is recognized as an essential micronutrient for both humans and animals to impede dental carries and facilitate the mineralization of hard tissues. Fluoride is beneﬁcial especially to young children below 8 years of age when present within allowable limits for calcination of dental enamel and bone formation . On the contrary, when the ﬂuoride concentration is high, it can act as a health hazards. The negatively charged ﬂuoride ion is highly attracted by positively charged ions, like calcium ions, of bones and teeth, which results in dental, skeletal and non skeletal ﬂuorisis [2,3]. Also it leads irregular formation of collagen, which serves as a major structural component of skin, ligaments, tendons, muscles, cartilage, bones and teeth. Most evidence indicates that ﬂuoride can interfere with DNA synthesis . The high concentrations of ﬂuoride can also interfere with carbohydrates, lipids, proteins, vitamins and mineral metabolism. Fluoride disperses to the environment through water, food, drugs, cosmetics and several engineering process such as semiconductor manufacturing, coal power plants, glass and ceramic production, uranium reﬁnement, electroplating, rub-
∗ Corresponding author. Tel.: +90 352 4374933; fax: +90 352 4374933. E-mail addresses: [email protected]
, [email protected]
(M. Soylak). 0304-3894/$ – see front matter © 2009 Elsevier B.V. All rights reserved. doi:10.1016/j.jhazmat.2009.02.109
ber, fertilizer manufacturing and natural sources [5,6]. According to the World Health Organization (WHO) the maximum allowable concentration of ﬂuoride is 1.5 mg L−1 . For these reasons, the removal of the excess ﬂuoride from waters and wastewaters is important in terms of protection of public health and environment. Deﬂuoridation of drinking water is the only practicable way to overcome the problem of excessive ﬂuoride in drinking water. Several treatment technologies, based on the principle of ion exchange , precipitation-coagulation , membrane processes such as reverse osmosis , Donnan dialysis , electrodialyses , nano-ﬁltration  have been developed for the removal of ﬂuoride from waters and wastewaters. Among the traditional methods; ion exchange method is a reliable way to remove ﬂuoride from water supplies but the efﬁciency of the method is reduced in presence of other ions like sulfate, carbonate, phosphate and alkalinity. Also this technique is expensive due to high cost of the resins. In precipitation-coagulation method, alum is the most commonly used coagulant. By using this process, only a smaller portion of ﬂuoride can remove in the form of precipitates and converts a greater portion of ionic ﬂuoride into soluble aluminium ﬂuoride complex ion. The soluble aluminium ﬂuoride complex is itself toxic so this technique is not desirable for deﬂuoritation of water. Although the membrane process is highly effective for ﬂuoride removal, by using this technique all the ions present in waters can remove, though some minerals are essential for living organisms and also this technique is very expensive [14,15].
B. Kemer et al. / Journal of Hazardous Materials 168 (2009) 888–894
Among the different wastewater treatment techniques, adsorption is one of the most popular separation and puriﬁcation method due to its high selectivity, easy handling, lower operating cost, high efﬁciency in reducing quantity of chemical and biological sludge and regeneration of adsorbents . Adsorption is a process where a solid is used for removing a soluble substance from water. The adsorption process consists of several mechanisms including chemisorption by ion exchange, complexation, coordination, chelating, physical adsorption and microprecipitation . The efﬁciency of the adsorption technique mainly depends on the nature of the adsorbents, so new, easy available, and high loading capacity adsorbents having a strong afﬁnity for understudy ion are needed. Several adsorbents were tried for the removal of ﬂuoride from waters and wastewaters namely activated alumina , activated carbon , calcite , clay , and hydrated cement , etc. In this study we have used a waste mud as an adsorbent, which was obtained from a Cu–Zn mine industry, for removal of ﬂuoride from aqueous solutions. The waste mud is one of the most promising adsorbent due to its zero price and easy availability. The waste mud emerges as an undesired by-product during the industrial applications. These wastes represent unused resources and in some cases serious disposal problems present so the utilization of waste mud for removal of impurities, is an important application. The aim of the present study was to evaluate the feasibility of using waste mud for removal of ﬂuoride ions from aqueous solutions. Three different forms of the waste mud were tested for their ﬂuoride removal performance: (i) original waste mud (o-WM), (ii) acid-treated waste mud (a-WM), and (iii) precipitated waste mud (p-WM). The residual ﬂuoride concentration in the aqueous phase was analyzed by using potentiometric method with a ﬂuoride ionselective electrode. Ion-selective electrodes (ISE) are the chemical sensors with the longest and probably the most frequent routine application. Potentiometric detection based on ion-selective electrodes, as a simple method, offers several advantages such as speed and ease of preparation and procedures, simple instrumentation, relatively fast response, wide dynamic range, reasonable selectivity, and low cost. Besides, they are ideally suitable for on-site analysis and, nowadays, they are found to be applicable in the analysis of some biologically relevant ions, process control, and environmental analysis [22,23]. The present study includes an observation of the effects of several experimental parameters such as contact time, initial pH of the solution, initial ﬂuoride concentration, waste mud concentration etc. The Langmuir and Freundlich isotherm models were used to describe equilibrium data. The adsorption mechanisms of ﬂuoride on the waste mud were also evaluated in terms of thermodynamics and kinetics. 2. Materials and methods 2.1. Preparation of different types of activated waste mud The waste mud was obtained from Cu–Zn mine-industry in C¸ayeli, Rize/Turkey (Inmet Mine Corp. Canada). The chemical composition of waste mud is 11.7% SiO2 , 8.9% Al2 O3 , 48.4% Fe2 O3 , 0.7% ZnO, 0.7% CuO and 29.6% other constituents . The composition of waste mud was determined by a ﬂame atomic absorption spectrometer (Unicam AA-929) for Al, Fe, Zn and Cu, and silica content was determined gravimetrically. The activation of waste mud by different techniques is considered as an effective way for increasing the speciﬁc surface area of waste mud. Therefore the waste mud activated with different methods was used in this study in order to evaluate their ﬂuoride removal performance. The o-WM was prepared by washing several times with distilled/ deionized water and dried at 110 ◦ C for 2 days. The a-WM was
prepared by reﬂuxing 10 g of water-washed and dried waste mud with 200 mL of 20% HCl solution for 2 h. After activation, the content was ﬁltered through 0.45 m nitrocellulose membrane (Sartorius Stedim Biotech. GmbH). The ﬁltrate was kept for preparing the precipitated waste mud. The obtained solid was washed several times with deionized water and dried 110 ◦ C for 2 days. For preparing the p-WM, the reﬂux solution which was obtained from acid activation was cooled to room temperature, and then the 25% ammonia solution was added drop by drop until complete precipitation. Then the precipitate was ﬁltered and washed thoroughly several times with deionized water until free from ammonia. The obtained solid was dried at 110 ◦ C for 2 days . 2.2. Adsorption experiments All chemicals and reagents used were of analytical reagent grade. All glassware and sample bottles were soaked in diluted HNO3 solution for 24 h and washed three times with deionized water. The NaF (Merck) was used for preparation of standard ﬂuoride stock solution (5000 mg L−1 ). The required concentration of ﬂuoride solution was prepared by appropriate dilutions of the stock solutions. Distilled/deionized water was used for all dilutions. The pH of the solutions was adjusted to the desired value with 0.1 M HCl and NaOH solutions. The adsorption experiments were carried out by batch technique. For this, 10 mL of ﬂuoride solutions in the concentration range of 5–950 mg L−1 were transferred into a polyethylene centrifuge tube. Then 10–200 mg of adsorbent (1–20 g L−1 ) were added to the solution, and the mixture was agitated on a mechanical shaker (Edmund Bühler GmbH) at 400 rpm for 4.0 h. After reaching the equilibrium, the adsorbent was removed by vacuum ﬁltration through 0.45 m nitrocellulose membrane. The ﬂuoride concentration in the supernatant was analyzed electrochemically with a ﬂuoride ion-selective electrode (Mettler Toledo DX219, dynamic range: 10−1 –10−6 M) by use of total ionic strength adjustment buffer (TISAB) solution (58 g of sodium chloride, 57 mL of glacial acetic acid and approximately 150 mL of 6 M NaOH in a volume of 1000 mL) to maintain pH 5.0 and to eliminate the interference effect of complexing ions. The ﬂuoride samples and the ﬂuoride standard solutions were diluted 1:1 with a total ionic strength adjustment buffer solution . All experiments were conducted in triplicate and the averages of the results were used for data analysis. 2.3. Adsorption kinetics The kinetics of adsorption is an important parameter from the point of view that it offers signiﬁcant insights into the adsorption mechanisms and reaction pathways. Several kinetic models have been developed to predict the adsorption kinetics and rate controlling step. In order to evaluate the kinetics of ﬂuoride adsorption on the p-WM, pseudo-ﬁrst-order, pseudo-second-order and intraparticle diffusion models were checked. The pseudo-ﬁrst-order Lagergren model is expressed as ; dQ = k1 (Qe − Qt ) dt
where Qe (mg g−1 ) and Qt (mg g−1 ) are the amounts of the ﬂuoride adsorbed on the adsorbate at equilibrium and at any time t, respectively; and k1 (min−1 ) is the rate constant of the ﬁrst order adsorption. After integration and applying boundary conditions Qt = 0 at t = 0 and Qt = Qt at t = t the integrated form of Eq. (1) becomes; ln(Qe − Qt ) = ln Qe − k1 t
The value of k1 and Qe can be obtained from the slope and intercept of the linear plot of ln(Qe –Qt ) versus t, respectively.
B. Kemer et al. / Journal of Hazardous Materials 168 (2009) 888–894
The second-order-kinetic model can be written as following form ; dQ = k2 (Qe − Qt )2 dt (g mg−1
(3) ln Qe = ln Kf +
is the rate constant of the second-order where k2 equation; Qe (mg g−1 ) is the maximum adsorption capacity; Qt (mg g−1 ) is the amount of adsorption at time t (min). After deﬁnite integration by applying the conditions Qt = 0 at t = 0 and Qt = Qt at t = t the Eq. (3) becomes the following; t 1 t = + Qt Qe k2 Qe 2
where Kf (mg g−1 ) and n are Freundlich constants related to adsorption capacity and intensity, respectively. The Freundlich model in linear form; 1 ln Ce n
The Freundlich constants Kf and 1/n are determined from the intercept and slope of linear plot of ln Qe versus ln Ce , respectively. 2.5. Adsorption thermodynamics
The value of Qe and k2 can be obtained from the slope and intercept of the linear plot of t/Qt versus t, respectively. The intraparticle diffusion equation is expressed as ;
In order to decide the feasibility and spontaneity of the adsorption process the thermodynamic parameters including Gibbs free energy change (G◦ ), enthalpy change (H◦ ), and entropy change (S◦ ) were evaluated. These parameters can be calculated using the following equations ;
Qt = kid t 1/2 + c
G◦ = −RT ln Kd
G◦ = H ◦ − TS ◦
where Qt (mg g−1 ) is the amount of adsorption at time t (min) and kid (mg g−1 min−1/2 ) is the rate constant of intraparticle diffusion. The value of kid and c can be determined the slope and intercept of the plot of Qt versus t1/2 , respectively. 2.4. Adsorption isotherms Adsorption isotherms are one of the most signiﬁcant tools to predict the adsorption capacity of the adsorbent and the mechanism of the adsorption. In order to evaluate the relationship between the amount of adsorbed ﬂuoride and the ﬂuoride concentration remaining in solution, two well known isotherm models are selected in this study; Langmuir and Freundlich isotherms. The Langmuir isotherm model assumes that the surface of the adsorbent is uniform, that is, all the adsorption sites are equivalent and adsorbed molecules do not interact. It also predicts all the adsorption occurs through the same mechanism. The Langmuir isotherm model commonly expressed as ; bQmax Ce Qe = 1 + bQmax
where Qe (mg g−1 ) is the amount of the ﬂuoride adsorbed per unit mass of adsorbent, Ce (mg L−1 ) is the equilibrium ﬂuoride concentration in the solution, Qmax (mg g−1 ) is the Langmuir constant related the maximum monolayer adsorption capacity and b (L mg−1 ) is the constant related the free energy or net enthalpy of adsorption. The Langmuir model in linear form; Ce Ce 1 = + Qmax Qe bQmax
This equation can be written as; ln Kd =
S ◦ H ◦ − R RT
where R is the universal gas constant (8.314 J mol−1 K−1 ), T is the temperature (K), and Kd is the distribution coefﬁcient. The Kd value was calculated using following equation; Kd = Qe /Ce
where Qe and Ce are the equilibrium concentration of ﬂuoride ions on adsorbent and in the solution, respectively. The values of H◦ and S◦ can be obtained from the slope and intercept of the plot of ln Kd versus 1/T, respectively. 3. Results and discussion 3.1. Effect of pH The pH of aqueous solution usually plays an important role in deciding the amount of ﬂuoride adsorbed on WM. The inﬂuence of aqueous phase pH on the uptake of ﬂuoride ions was investigated by using three types of WM; o-WM, a-WM and p-WM. Adsorption experiments were carried out at various aqueous phase pH (2.0–8.0) by keeping all other experimental conditions constant
The plot of Ce /Qe versus Ce gives a straight line and the values of Qmax and b can be calculated from the slope and intercept of the plot, respectively. In order to evaluate the feasibility of the process, the Langmuir isotherm can be described in terms of the dimensionless constant; separation factor or equilibrium parameter , RL =
1 1 + bCo
where b (L mg−1 ) is the Langmuir isotherm constant and Co (mg L−1 ) is the initial concentration of ﬂuoride. There are four probabilities for the RL value: (i) for favorable adsorption 0 < RL < 1, (ii) for unfavorable adsorption RL > 1, (iii) for linear adsorption RL = 1 and (iv) for irreversible adsorption RL = 0. The Freundlich isotherm model is based on the adsorption on heterogeneous surfaces and is presented by the following equation ; Qe = Kf Ce
Fig. 1. Effect of initial pH on ﬂuoride uptake by three types of waste mud (initial F− concentration: 80 mg L−1 , waste mud concentration: 10 g L−1 , contact time: 1 h, temperature: 20 ± 1 ◦ C).
B. Kemer et al. / Journal of Hazardous Materials 168 (2009) 888–894
(shaking time; 1 h, adsorbent concentration; 10 g L−1 ; initial ﬂuoride concentration; 80 mg L−1 ). The ﬂuoride uptake capacity is not affected in the pH range of 2.0–8.0 for all the types of WM so it can be concluded that the present adsorption process is not pH-dependent [34,35]. Furthermore the maximum ﬂuoride uptake was obtained
Table 1 Freundlich and Langmuir isotherm constants and correlation coefﬁcients for the adsorption of ﬂuoride on three types of WM. Type of WM
p-WM a-WM o-WM
Qmax (mg g−1 )
b (L mg−1 )
Kf mg g−1 )
27.2 2.8 4.2
0.01544 0.00866 0.00913
0.993 0.989 0.997
1.22 10.79 7.95
2.290 2.02 2.13
0.974 0.986 0.964
with p-WM (Fig. 1). Hence all subsequent studies were conducted with p-WM at pH 5.0. 3.2. The ﬂuoride removal performance of different types of waste mud In order to decide the best type of waste mud for ﬂuoride uptake, the linearized Langmuir and Freundlich isotherms were obtained for three types of waste mud, o-WM, a-WM, and p-WM. The adsorption process was conducted with initial ﬂuoride ions concentrations between 5.0 and 950 mg L−1 and different types of waste mud concentration of 10 g L−1 at pH 5.0 and equilibrium time of 1 h. The Langmuir and Freundlich isotherms were plotted as a function of different types of waste mud (Fig. 2(a), (b) and (c)), and the values of isotherm constants and correlation coefﬁcients were calculated for both isotherm models (Table 1) by using the data obtained from these ﬁgures. The highest value of Qmax obtained from Langmuir model for p-WM is 27.2 mg g−1 with a high correlation coefﬁcient of 0.99. It appears to be the highest in comparison with the uptake obtained by using other type of waste mud. 3.3. The effect of contact time and kinetics of adsorption In order to obtain an appropriate contact time between the p-WM and ﬂuoride ions, the adsorption experiments were carried out by conducting 97.2 mg L−1 of ﬂuoride solutions at initial pH 5.0 with 10 g L−1 of p-WM suspensions. The mixtures were agitated at 400 rpm. The samples were taken different periods of time and analyzed for their ﬂuoride concentration. The results showed that a contact time of 60 min was adequate to reach equilibrium and there was no signiﬁcant increase in the rate of removal with further increase in contact time (Fig. 3). This may be due to the
Fig. 2. Removal performance of three type of WM (a) Ce versus Qe graph (b) Langmuir isotherm model, (c) Freundlich isotherm model (initial pH: 5.0, initial ﬂuoride conc.: 5.4–914 mg L−1 , contact time: 1 h, WM conc.: 10 g L−1 , temperature: 20 ± 1 ◦ C).
Fig. 3. Effect of contact time on ﬂuoride uptake (initial pH: 5.0, initial ﬂuoride conc.: 97.2 mg L−1 , p-WM conc.: 10 g L−1 , temperature: 20 ± 1 ◦ C).
B. Kemer et al. / Journal of Hazardous Materials 168 (2009) 888–894
Table 2 Parameters of pseudo-ﬁrst-order, pseudo-second-order and intraparticle diffusion models at 20 ± 1 ◦ C. Exp. Qe (mg g−1 )
k1 (min 7.33
Qe (mg g −3
−7.90 × 10
k2 (g mg
Intraparticle diffusion Qe (mg g 7.32
kid (mg g−1 min−1/2 )
C (mg g−1 )
larger surface area of the p-WM is available at the beginning for the adsorption of ﬂuoride. The kinetics of ﬂuoride adsorption on the p-WM was determined by using three different kinetic models, which are pseudo-ﬁrstorder, pseudo-second-order and intraparticle diffusion models. The pseudo-ﬁrst-order rate constant (k1 ) and theoretical equilibrium adsorption capacities (Qe ) calculated from linear plot of ln (Qe –Qt ) versus t, are given in Table 2. The value of correlation coefﬁcient is extremely low (0.294) and also Qe,cal determined from the model is not in a good agreement with the experimental values of Qe,exp . Therefore it could be said that the adsorption of ﬂuoride on the p-WM does not follow the pseudo-ﬁrst-order kinetic model. The graph of t/Qt versus t for the linear pseudo-second-order model was plotted, and the second order rate constant k2 and maximum adsorption capacity Qe were calculated from the intercept and slope of this graph, respectively (Table 2). The correlation coefﬁcient value is magniﬁcent (1.00), and the equilibrium adsorption capacity Qe,cal (7.32 mg g−1 ) determined by using the second order model is nearly as same as with the experimentally determined equilibrium adsorption capacity Qe,exp (7.33 mg g−1 ). The intraparticle rate constant (kid ) and c parameters obtained from the plots of Qt versus t1/2 for the intraparticle diffusion model are given in Table 2. The value of c obtained from intraparticle diffusion model is not zero and the correlation coefﬁcient is not satisfactory (0.436), indicating that the intraparticle diffusion may not be the controlling factor in determining the kinetics of the process. As a result, it can be said that the pseudo-second-order kinetic model suggested a good correlation for the adsorption of ﬂuoride on the p-WM in contrast to the pseudo-ﬁrst-order model and intraparticle diffusion model, so pseudo-second-order model is suitable for modeling the adsorption of ﬂuoride on the p-WM. 3.4. The effect of p-WM and ﬂuoride concentration on ﬂuoride uptake The effect of p-WM and initial ﬂuoride concentration on the removal of ﬂuoride from aqueous solutions was studied with initial ﬂuoride concentration between 26.2–565 mg L−1 and p-WM concentrations in the range of 1–20 g L−1 for 1.0 h contact time at pH 5.0. In order to evaluate the adsorption capacity of p-WM, the equilibrium data for the adsorption of ﬂuoride were analyzed in the light of adsorption isotherms. Fig. 4(a) and (b) depicts the Freundlich and Langmuir isotherm models, respectively. It is evident from the results, as the concentration of p-WM increased; the equilibrium ﬂuoride uptake increased however the percent amount of the adsorbed ﬂuoride ions decreases with increase in the ﬂuoride concentration which indicated that the adsorption depends upon the availability of binding sites for ﬂuoride ions. The values of isotherm parameters and correlation coefﬁcients obtained from the slope and intercept of the plots of each isotherm models are given in Table 3. Both of the adsorption isotherms were deﬁned as suitable models for the adsorption of ﬂuoride ions on the pWM because the correlation coefﬁcients were satisfactory (in the range 0.964–0.998), indicating that the homogenous and heterogeneous distribution of active sites on the surface of p-WM. The RL value ranges from 0.67 to 0.08 for the initial ﬂuoride concentration in the range of 26.2–565 mg L−1 at a constant p-WM concentration (10 g L−1 ). This parameter indicated that the p-WM is a suitable adsorbent for the adsorption of ﬂuoride ions from aqueous
Fig. 4. Effect of p-WM concentration on ﬂuoride uptake (a) Freundlich isotherm model, (b) Langmuir isotherm model (initial pH: 5.0, initial ﬂuoride conc.: 26.2–565 mg L−1 , contact time: 1 h, p-WM conc.: 10 g L−1 , temperature: 20 ± 1 ◦ C).
Table 3 Freundlich and Langmuir isotherm constants and correlation coefﬁcients for the adsorption of ﬂuoride on p-WM at various p-WM concentrations at pH 5.0. p-WM conc. (g L−1 )
1.0 5.0 7.5 10.0 15.0
Qmax (mg g−1 )
b (L mg−1 )
Kf (mg g−1 )
46.7 31.7 31.0 26.5 20.7
0.00784 0.01230 0.01234 0.01971 0.02460
0.972 0.967 0.964 0.993 0.992
2.09 1.46 1.10 1.22 1.04
2.14 2.00 1.79 1.83 1.81
0.998 0.998 0.995 0.987 0.983
B. Kemer et al. / Journal of Hazardous Materials 168 (2009) 888–894
Table 4 Thermodynamic parameters of the ﬂuoride adsorption on the p-WM at different temperatures. T (◦ C)
S◦ (J/mol K)a
0 10 20 30 40
−2.06 −2.35 −2.97 −3.42 −3.95
Measured between 273 and 313 K.
solutions. Also the values of 1/n lying between 0.47 and 0.55 (1.04–2.09 for n values) suggested that the adsorption process was favorable under studied conditions. 3.5. The effect of temperature and thermodynamic parameters of adsorption In order to evaluate the effect of temperature on the uptake of ﬂuoride ions, the adsorption experiments were conducted in the temperature range of 0–40 ◦ C with p-WM concentration of 10 g L−1 and initial ﬂuoride concentration of 200 mg L−1 at initial pH 5.0. In order to control the temperature of the solutions, a cryostat (Nüve BD 402, temperature range: −10 to +40 ◦ C) was used for all thermodynamic studies. The results indicated that the percentage removal of ﬂuoride increased from 71.3% to 82.0% when the temperature was increased from 0 to 40 ◦ C. The increase in adsorption capacity of p-WM with temperature may be attributed to increase in the number of available active surface sites for adsorption on the p-WM. The values of G◦ , H◦ , and S◦ for the adsorption of ﬂuoride ions on the p-WM at different temperature are given in Table 4. The negative values of G◦ indicated that the adsorption process was spontaneous at all temperatures studied. The entropy change (S◦ ) and enthalpy change (H◦ ) for the adsorption process were calculated to be 48.22 J mol−1 K−1 and 11.18 kJ mol−1 , respectively. The positive value of H◦ suggested the endothermic nature of adsorption. The endothermic nature may be also predicted from the increase in value of ﬂuoride uptake of the p-WM with the rise in temperature. The magnitude of H◦ gives an idea about the type of sorption. Adsorption can be either physical or chemical in nature. Chemical adsorption occurs usually at higher temperatures than those at which physical adsorption occurs; furthermore, chemical adsorption is ordinarily a slower process than physical adsorption and, like most chemical reactions, frequently involves an energy of activation. The enthalpy for physical adsorption is usually no more than 1 kcal mol−1 (4.2 kJ mol−1 ) and for chemical adsorption is more than 5 kcal mol−1 (21 kJ mol−1 )  so it seems that adsorption of ﬂuoride ions on the p-WM is almost a chemical process. The positive value of S◦ suggested an increase in randomness at the solid/solution interface during the adsorption process and a good afﬁnity of ﬂuoride with p-WM.
Fig. 5. Reuse of the p-WM without regeneration (initial pH: 5.0, initial ﬂuoride conc.: 92.5 mg L−1 , contact time: 1 h, p-WM conc.: 10 g L−1 , temperature: 20 ± 1 ◦ C).
compared to the ﬁrst three cycles. Similar behavior was reported by previous researchers . From the results, the p-WM can be used at least ﬁve times without regeneration. 3.7. The effect of some common ions over the adsorption yields of ﬂuoride The ﬂuoride-contaminated drinking and wastewater contain several other co-existing ions such as nitrate, sulfate and phosphate, which can compete with ﬂuoride ions during the adsorption process for the active sites on the p-WM. Hence the effect of these competitive ions on the uptake of ﬂuoride ions should be studied. The anion (NO3 − , SO4 2− , and PO4 3− ) solutions were prepared by dissolving appropriate amount of their sodium salts. Adsorption experiments were carried out by adding 100 mg L−1 of NO3 − , SO4 2− , PO4 3− and mixture of these ions, individually, in 80 mg L−1 of ﬂuoride solution containing 10 g L−1 of p-WM. Fig. 6 shows the effect of various co-existing ions on ﬂuoride adsorption by p-WM. From the
3.6. Reuse of the p-WM without regeneration In order to evaluate the reusability of the p-WM without regeneration, the adsorption experiments were conducted by using an initial ﬂuoride concentration of 92.5 mg L−1 at pH 5.0 with 10 g L−1 of p-WM for 1 hour of contact time. The p-WM loaded with ﬂuoride ions was ﬁltered, air dried and transferred to another 92.5 mg L−1 of ﬂuoride solution. This process was repeated for ﬁve times. After ﬁrst cycle the adsorbed amount of ﬂuoride was 7.0 mg g−1 and after each adsorption process, the adsorption capacity of p-WM was decreased as shown in Fig. 5. After cycle 4 and 5, the newly adsorbed amount of ﬂuoride were 1.1 and 0.5 mg g−1 , respectively indicating that the amount of ﬂuoride removal signiﬁcantly decreased
Fig. 6. Effect of some common anions on the ﬂuoride uptake (initial pH: 5.0, p-WM conc.: 10 g L−1 , initial anions conc.: 100 mg L−1 , initial ﬂuoride conc.: 80 mg L−1 ).
B. Kemer et al. / Journal of Hazardous Materials 168 (2009) 888–894
results, nitrate, sulfate and phosphate had no signiﬁcant interfere effect on the adsorption of ﬂuoride. 4. Conclusion The results exhibit that the p-WM, which was obtained from Cu–Zn mine (C¸ayeli, Rize/Turkey) is a promising material to remove excess ﬂuoride from waters and wastewaters. The utilization of p-WM is a signiﬁcant application because it has been produced from an industrial waste material so these wastes represent unused resources and also present serious disposal problems. The adsorption process was independent of pH for all types of waste mud. Maximum ﬂuoride uptake was obtained with p-WM. The kinetic study indicated that adsorption of ﬂuoride was very rapid, and the equilibrium was reached within 60 min at room temperature. Adsorption kinetics followed pseudo-second-order model with an excellent correlation coefﬁcient value of 1.00. The equilibrium data are best ﬁtted to the Langmuir and Freundlich isotherm models with R2 value of higher than 0.9, indicating that the homogenous and heterogeneous distribution of active sites on the surface of p-WM. The negative value of G◦ and positive value S◦ showed that the adsorption of ﬂuoride ions on the p-WM was feasible and spontaneous. And also the positive value of entropy change suggested an increase in randomness. The positive value of H◦ conﬁrmed the endothermic nature of adsorption. Some common ions which exist in drinking and wastewater had no signiﬁcant interfere effect on adsorption of ﬂuoride. The p-WM can be used at least ﬁve times for further adsorption process without regeneration. The results obtained from the present study demonstrated that the p-WM can be used as a no cost, highly effective and easy available adsorbent for removal of ﬂuoride from aqueous solutions. Acknowledgements Authors thank to the Unit of the Scientiﬁc Research Projects of Karadeniz Technical University for the ﬁnancial support. Authors also thank Prof. H. Basri Senturk for allowing use of his laboratory facilities. References  M. Srimurali, A. Pragathi, J. Karthikeyan, A study on removal of ﬂuorides from drinking water by adsorption onto low-cost materials, Environ. Pollut. 99 (1998) 285–289.  S.V. Mohan, S.V. Ramanaiah, B. Rajkumar, P.N. Sarma, Biosorption of ﬂuoride from aqueous phase onto algal Spirogyra IO1 and evaluation of adsorption kinetics, Bioresour. Technol. 98 (2007) 1006–1011.  A.K. Susheela, A. Kumar, M. Betnagar, M. Bahadur, Prevalence of endemic ﬂuorosis with gastro-intestinal manifestations in people living in some North-Indian villages, Fluoride 26 (1993) 97–104.  T. Tsutsui, N. Suzuki, M. Ohmori, H. Maizumi, Cytotoxicity, chromosome aberrations and unscheduled DNA synthesis in cultured human diploid ﬁbroblasts induced by sodium ﬂuoride, Mutat. Res. Apr. 139 (1984) 193–198.  E. Oguz, Equilibrium isotherms and kinetics studies for the sorption of ﬂuoride on light weight concrete materials, Colloids Surf. A: Physicochem. Eng. Aspects. 295 (2007) 258–263.  K. Sarala, P.R. Rao, Endemic ﬂuorosis in the Village Ralla, Anantapuram in Andhra Pradesh – an epidemiological study, Fluoride 26 (1993) 177–180.  WHO (World Health Organization), Guidelines for Drinking Water Quality (vol. II): Health Criteria and Supporting Information, World Health Organization, Geneva, Switzerland, 1984.
 L. Ruixia, G. Jinlong, T. Hongxiao, Adsorption of ﬂuoride, phosphate, and arsenate ions on a new type of ion exchange ﬁber, J. Colloid Interface Sci. 248 (2002) 268–274.  S. Saha, Treatment of aqueous efﬂuent for ﬂuoride removal, Water Res. 27 (1993) 1347–1350.  S.V. Joshi, S.H. Mehta, A.P. Rao, A.V. Rao, Estimation of sodium ﬂuoride using HPLC in reverse osmosis experiments, Water Treat. 10 (1992) 307–312.  M. Hichour, F. Persin, J. Sandeaux, C. Gavach, Fluoride removal from waters by Donnan dialysis, Sep. Purif. Technol. 18 (2000) 1–11.  S.K. Adhikary, U.K. Tipnis, W.P. Harkare, K.P. Govindan, Deﬂuoridation during desalination of brackish water by electrodialysis, Desalination 71 (1989) 301–312.  R. Simons, Trace element removal from ash dam waters by nanoﬁltration and diffusion dialysis, Desalination 89 (1993) 325–341.  R.C. Meenakshi, Maheshwari, Fluoride in drinking water and its removal, J. Hazard. Mater. 137 (2006) 456–463.  B.V. Apparao, G. Kartikeyan, Permissible limits of ﬂuoride on in drinking water in India in rural environment, Ind. J. Environ. Protec. 6 (1986) 172–175.  P. King, N. Rakesh, S. Beenalahari, Y.P. Kumar, V.S.R.K. Prasad, Removal of lead from aqueous solution using Syzygium cumini L.: equilibrium and kinetic studies, J. Hazard. Mater. 142 (2007) 340–347.  B. Volesky, Detoxiﬁcation of metal-bearing efﬂuents: biosorption for the next century, Hydrometallurgy 59 (2001) 203–216.  J.F. Rubel, The removal of excess ﬂuoride from drinking water by the activated alumina method, in: J.L. Shupe, H.P. Peterson, N.C. Leone (Eds.), Fluoride Effects on Vegetation Animals and Humans, Paragon Press, Salt Lake City, 1983, pp. 345–349.  S. Al-Asheh, F. Banat, L. Abu-Aitah, Adsorption of phenol using different types of bentonite, Sep. Purif. Technol. 33 (2003) 1–10.  S. Meenakshi, C.S. Sundaram, R. Sukumar, Enhanced ﬂuoride sorption by mechano-chemically activated kaolinites, J. Hazard. Mater. 153 (2008) 164–172.  S. Kagne, S. Jagtap, P. Dhawade, S.P. Kamble, S. Devotta, S.S. Rayalu, Hydrated cement: a promising adsorbent for the removal of ﬂuoride from aqueous solution, J. Hazard. Mater. 154 (2008) 88–95.  B. Kemer, M. Ozdemir, Potentiometric utility of the new solid-state sensor based on crowned ionophore for the determination of K+ , Turk. J. Chem. 32 (2008) 521–528.  S. Kim, H. Kim, K.H. Noh, S.H. Lee, S.K. Kim, J.S. Kim, Potassium ion-selective membrane electrodes based on 1,3-alternate calixcrown-5-azacrown-5, Talanta 61 (2003) 709–716.  D. Ozdes, A. Gundogdu, B. Kemer, C. Duran, H.B. Senturk, M. Soylak, Removal of Pb(II) ions from aqueous solution by a waste mud from copper mine industry: equilibrium, kinetic and thermodynamic study, J. Hazard. Mater. 2009, in press, doi:10.1016/j.jhazmat.2008.12.073.  J. Pradhan, J. Das, S. Das, R.S. Thakur, Adsorption of phosphate from aqueous solution using activated red mud, J. Coll. Interf. Sci. 204 (1998) 169–172.  J.H. Kennedy, Analytical Chemistry Principles, second ed., W.B. Saunders Company, New York, 1990.  S. Lagergren, About the theory of so-called adsorption of soluble substance, Kung Sven. Veten. Hand 24 (1898) 1–39.  Y.S. Ho, G. McKay, Kinetic models for the sorption of dye from aqueous solution by wood, J. Environ. Sci. Health Part B: Process Saf. Environ. Prot. 76 (1998) 183–191.  W.J. Weber Jr., J.C. Morriss, Kinetics of adsorption on carbon from solution, J. Sanitary Eng. Div. Am. Soc. Civ. Eng. 89 (1963) 31–60.  M.J. Angove, B.B. Johson, J.D. Wells, Adsorption of cadmium(II) on kaolinite, Colloid Surf. A: Phys. Eng. Aspects 126 (1997) 137–147.  T.W. Weber, R.K. Chakravorti, Pore and solid diffusion models for ﬁxed bed adsorbers, J. Am. Inst. Chem. Eng. 20 (1974) 228–238.  H.M.F. Freundlich, Über die adsorption in lösungen, Z. Phys. Chem. 57 (1906) 385–470.  C. Raji, T.S. Anirudhan, Kinetics of Pb(II) adsorption by polyacrylamide grafted sawdust, Indian J. Chem. Technol. 4 (1997) 157–162.  W. Nigussie, F. Zewge, B.S. Chandravanshi, Removal of excess ﬂuoride from water using waste residue from alum manufacturing process, J. Hazard. Mater. 147 (2007) 954–963.  N. Viswanathan, C.S. Sundaram, S. Meenakshi, Removal of ﬂuoride from solution using protonated chitosan beads, J. Hazard. Mater. 161 (2009) 423–430.  M. Khormaei, B. Nasernejad, M. Edrisi, T. Eslamzadeh, Copper biosorption from aqueous solutions by sour orange residue, J. Hazard. Mater. 149 (2007) 269–274.  H. Serencam, A. Gundogdu, Y. Uygur, B. Kemer, V.N. Bulut, C. Duran, M. Soylak, M. Tufekci, Removal of cadmium from aqueous solution by Nordmann ﬁr (Abies nordmanniana (Stev.) Spach. Subsp. nordmanniana) leaves, Bioresour. Technol. 99 (2008) 1992–2000.